#------------------------------------------------------------------------------
#$Date: 2016-02-16 02:10:39 +0100 (Tue 16 de Feb de 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/18/7021887.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7021887
loop_
_publ_author_name
'Liu, Ding'
'Lu, Ying'
'Li, Yang-Guang'
'Tan, Hua-Qiao'
'Chen, Wei-Lin'
'Zhang, Zhi-Ming'
'Wang, En-Bo'
_publ_section_title
;
 Assembly of trimeric polyoxovanadate aggregates based on [MnV13O38](7-)
 building blocks and lanthanide cations.
;
_journal_issue                   40
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              14445
_journal_page_last               14453
_journal_paper_doi               10.1039/c3dt51250a
_journal_volume                  42
_journal_year                    2013
_chemical_formula_sum            'C18 H109.5 Ce6 K1.5 Mn3 N3 O172.5 S2 V39'
_chemical_formula_weight         6243.56
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   24.707(4)
_cell_length_b                   24.707(4)
_cell_length_c                   17.215(3)
_cell_measurement_reflns_used    5525
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      3.04
_cell_volume                     9101(3)
_computing_cell_refinement       'SAINT (Bruker, 1999)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID IP'
_diffrn_measurement_method       Oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0916
_diffrn_reflns_av_unetI/netI     0.0422
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            65771
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         3.04
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.737
_exptl_absorpt_correction_T_max  0.423
_exptl_absorpt_correction_T_min  0.365
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8 March, 1995'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.278
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             5998
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.23
_platon_squeeze_details
;
;
_refine_diff_density_max         2.251
_refine_diff_density_min         -1.237
_refine_diff_density_rms         0.221
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.988
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     395
_refine_ls_number_reflns         5525
_refine_ls_number_restraints     61
_refine_ls_restrained_S_all      0.991
_refine_ls_R_factor_all          0.0905
_refine_ls_R_factor_gt           0.0689
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0500P)²+300.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1721
_refine_ls_wR_factor_ref         0.1831
_reflns_number_gt                4125
_reflns_number_total             5525
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3dt51250a.txt
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      P6(3)/m
_cod_original_formula_sum        'C18 H109.50 Ce6 K1.50 Mn3 N3 O172.50 S2 V39'
_cod_database_code               7021887
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.48920(3) 0.79948(3) 0.52426(5) 0.0400(2) Uani 1 1 d .
Mn1 Mn 0.66627(10) 0.86981(10) 0.7500 0.0211(5) Uani 1 2 d S
V3 V 0.51982(11) 0.81189(11) 0.7500 0.0221(5) Uani 1 2 d S
V4 V 0.58398(8) 0.74976(8) 0.65724(11) 0.0250(4) Uani 1 1 d .
V5 V 0.60719(8) 0.93371(8) 0.65737(11) 0.0261(4) Uani 1 1 d .
V6 V 0.75660(9) 0.98682(9) 0.65895(12) 0.0313(5) Uani 1 1 d .
V7 V 0.73466(9) 0.81580(10) 0.65866(12) 0.0311(5) Uani 1 1 d .
V8 V 0.66795(9) 0.87046(10) 0.56045(12) 0.0280(5) Uani 0.92 1 d P
V9 V 0.65203(14) 0.69266(13) 0.7500 0.0340(7) Uani 1 2 d S
V10 V 0.69802(14) 1.05386(13) 0.7500 0.0353(7) Uani 1 2 d S
O23 O 0.5553(4) 0.9011(4) 0.7500 0.023(2) Uani 1 2 d S
O22 O 0.5355(4) 0.7430(5) 0.7500 0.023(2) Uani 1 2 d S
O21 O 0.6035(3) 0.8449(3) 0.6737(4) 0.0228(15) Uani 1 1 d .
O20 O 0.4738(3) 0.7933(4) 0.6730(5) 0.0326(19) Uani 1 1 d .
O19 O 0.5876(4) 0.6832(3) 0.6742(5) 0.0321(18) Uani 1 1 d .
O18 O 0.6583(3) 0.7915(3) 0.5963(4) 0.0258(16) Uani 1 1 d .
O17 O 0.5525(4) 0.9081(3) 0.5916(5) 0.0313(18) Uani 1 1 d .
O16 O 0.6563(4) 0.7907(5) 0.7500 0.023(2) Uani 1 2 d S
O15 O 0.5302(3) 0.7316(4) 0.5924(5) 0.0308(18) Uani 1 1 d .
O14 O 0.6289(4) 1.0102(4) 0.6744(5) 0.0345(19) Uani 1 1 d .
O13 O 0.6770(5) 0.9493(5) 0.7500 0.025(2) Uani 1 2 d S
O12 O 0.6791(3) 0.9497(3) 0.5967(4) 0.0278(17) Uani 1 1 d .
O11 O 0.6032(4) 0.8445(4) 0.5078(5) 0.035(2) Uani 0.92 1 d P
O10 O 0.7503(4) 1.0562(3) 0.6730(5) 0.0348(19) Uani 1 1 d .
O9 O 0.7264(3) 0.8939(3) 0.6682(5) 0.0285(17) Uani 1 1 d .
O8 O 0.7094(4) 0.7334(4) 0.6733(5) 0.0346(19) Uani 1 1 d .
O7 O 0.8081(4) 1.0065(4) 0.5937(5) 0.044(2) Uani 1 1 d .
O6 O 0.7869(4) 0.8375(4) 0.5936(5) 0.043(2) Uani 1 1 d .
O5 O 0.7997(5) 0.9973(5) 0.7500 0.034(3) Uani 1 2 d S
O4 O 0.6431(6) 0.6246(6) 0.7500 0.052(4) Uani 1 2 d S
O3 O 0.7800(5) 0.8400(5) 0.7500 0.031(3) Uani 1 2 d S
O2 O 0.7242(4) 0.8929(4) 0.4991(5) 0.041(2) Uani 0.92 1 d P
O1 O 0.7072(7) 1.1224(5) 0.7500 0.048(3) Uani 1 2 d S
O5W O 0.3974(4) 0.6950(4) 0.5503(6) 0.050(3) Uani 1 1 d .
O4W O 0.5086(6) 0.7368(6) 0.4250(7) 0.081(4) Uani 1 1 d .
O3W O 0.4107(5) 0.8334(5) 0.5571(8) 0.073(3) Uani 1 1 d .
O2W O 0.5277(5) 0.8854(5) 0.4245(8) 0.076(4) Uani 1 1 d .
O1W O 0.4117(7) 0.7728(7) 0.4150(10) 0.111(5) Uani 1 1 d .
S1 S 0.3333 0.6667 0.5789(4) 0.0402(13) Uani 1 3 d S
O25 O 0.3333 0.6667 0.6629(12) 0.073(6) Uani 1 3 d S
OW2 O 0.0892(6) 0.1446(5) 0.4846(7) 0.073(3) Uani 1 1 d .
OW1 O 0.3405(6) 0.3541(6) 0.4520(7) 0.084(4) Uani 1 1 d .
O51 O 0.0997(7) 0.1628(8) 0.3157(8) 0.120(5) Uani 1 1 d DU
C1 C 0.1174(11) 0.1926(9) 0.2500 0.089(6) Uani 1 2 d SDU
C2 C 0.1584(10) 0.2602(8) 0.2500 0.089(5) Uani 1 2 d SDU
C4 C 0.2169(9) 0.3569(8) 0.3204(6) 0.115(5) Uani 0.50 1 d PDU
N1 N 0.2169(9) 0.3569(8) 0.3204(6) 0.115(5) Uani 0.50 1 d P
C3 C 0.1773(9) 0.2924(8) 0.3209(7) 0.100(5) Uani 1 1 d DU
C5 C 0.2364(16) 0.3899(9) 0.2500 0.130(7) Uani 1 2 d SDU
OW3 O 0.1130(6) 0.3905(6) 0.4512(8) 0.087(4) Uiso 1 1 d .
OW4 O 0.0281(14) 0.0491(13) 0.2500 0.056(7) Uiso 0.50 2 d SP
V11 V 0.8204(8) 0.9312(8) 0.7500 0.032(4) Uiso 0.17 2 d SP
O53 O 0.8836(19) 0.9562(19) 0.696(3) 0.024(9) Uiso 0.17 1 d P
O6W O 0.0000 0.0000 0.381(3) 0.085(13) Uiso 0.50 3 d SP
K1 K 0.3586(6) 0.7714(6) 0.7500 0.072(3) Uiso 0.50 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O11 Ce1 O5W 137.1(3) . .
O11 Ce1 O4W 70.9(4) . .
O5W Ce1 O4W 80.7(4) . .
O11 Ce1 O2W 71.1(3) . .
O5W Ce1 O2W 139.8(4) . .
O4W Ce1 O2W 87.0(5) . .
O11 Ce1 O1W 125.2(5) . .
O5W Ce1 O1W 71.5(4) . .
O4W Ce1 O1W 71.7(5) . .
O2W Ce1 O1W 68.3(4) . .
O11 Ce1 O3W 139.9(3) . .
O5W Ce1 O3W 81.4(3) . .
O4W Ce1 O3W 140.4(4) . .
O2W Ce1 O3W 84.4(4) . .
O1W Ce1 O3W 69.3(5) . .
O11 Ce1 O20 104.0(3) . .
O5W Ce1 O20 74.2(3) . .
O4W Ce1 O20 135.0(4) . .
O2W Ce1 O20 135.1(4) . .
O1W Ce1 O20 130.8(4) . .
O3W Ce1 O20 71.6(3) . .
O11 Ce1 O17 68.0(3) . .
O5W Ce1 O17 139.2(3) . .
O4W Ce1 O17 137.5(3) . .
O2W Ce1 O17 69.9(3) . .
O1W Ce1 O17 125.9(4) . .
O3W Ce1 O17 74.0(3) . .
O20 Ce1 O17 67.3(2) . .
O11 Ce1 O15 67.9(3) . .
O5W Ce1 O15 72.5(3) . .
O4W Ce1 O15 69.9(4) . .
O2W Ce1 O15 137.6(3) . .
O1W Ce1 O15 130.5(4) . .
O3W Ce1 O15 135.6(3) . .
O20 Ce1 O15 67.2(2) . .
O17 Ce1 O15 103.5(2) . .
O16 Mn1 O13 179.5(4) . .
O16 Mn1 O21 90.1(3) . .
O13 Mn1 O21 90.3(3) . .
O16 Mn1 O21 90.1(3) . 10_557
O13 Mn1 O21 90.3(3) . 10_557
O21 Mn1 O21 88.3(4) . 10_557
O16 Mn1 O9 90.0(3) . 10_557
O13 Mn1 O9 89.6(3) . 10_557
O21 Mn1 O9 176.7(3) . 10_557
O21 Mn1 O9 88.4(3) 10_557 10_557
O16 Mn1 O9 90.0(3) . .
O13 Mn1 O9 89.6(3) . .
O21 Mn1 O9 88.4(3) . .
O21 Mn1 O9 176.7(3) 10_557 .
O9 Mn1 O9 94.8(5) 10_557 .
O16 Mn1 V6 130.5(2) . 10_557
O13 Mn1 V6 49.1(2) . 10_557
O21 Mn1 V6 139.3(2) . 10_557
O21 Mn1 V6 92.5(2) 10_557 10_557
O9 Mn1 V6 40.7(2) 10_557 10_557
O9 Mn1 V6 89.8(2) . 10_557
O16 Mn1 V6 130.5(2) . .
O13 Mn1 V6 49.1(2) . .
O21 Mn1 V6 92.5(2) . .
O21 Mn1 V6 139.3(2) 10_557 .
O9 Mn1 V6 89.8(2) 10_557 .
O9 Mn1 V6 40.7(2) . .
V6 Mn1 V6 61.70(9) 10_557 .
O16 Mn1 V7 49.3(2) . .
O13 Mn1 V7 130.3(2) . .
O21 Mn1 V7 92.5(2) . .
O21 Mn1 V7 139.4(2) 10_557 .
O9 Mn1 V7 90.1(2) 10_557 .
O9 Mn1 V7 41.0(2) . .
V6 Mn1 V7 112.01(9) 10_557 .
V6 Mn1 V7 81.24(7) . .
O16 Mn1 V7 49.3(2) . 10_557
O13 Mn1 V7 130.3(2) . 10_557
O21 Mn1 V7 139.4(2) . 10_557
O21 Mn1 V7 92.5(2) 10_557 10_557
O9 Mn1 V7 41.0(2) 10_557 10_557
O9 Mn1 V7 90.1(2) . 10_557
V6 Mn1 V7 81.24(7) 10_557 10_557
V6 Mn1 V7 112.01(9) . 10_557
V7 Mn1 V7 61.85(9) . 10_557
O16 Mn1 V4 45.9(2) . .
O13 Mn1 V4 134.5(2) . .
O21 Mn1 V4 44.3(2) . .
O21 Mn1 V4 90.4(2) 10_557 .
O9 Mn1 V4 135.9(2) 10_557 .
O9 Mn1 V4 87.3(2) . .
V6 Mn1 V4 175.40(10) 10_557 .
V6 Mn1 V4 117.65(5) . .
V7 Mn1 V4 63.60(6) . .
V7 Mn1 V4 95.11(8) 10_557 .
O16 Mn1 V4 45.9(2) . 10_557
O13 Mn1 V4 134.5(2) . 10_557
O21 Mn1 V4 90.4(2) . 10_557
O21 Mn1 V4 44.3(2) 10_557 10_557
O9 Mn1 V4 87.3(2) 10_557 10_557
O9 Mn1 V4 135.9(2) . 10_557
V6 Mn1 V4 117.65(5) 10_557 10_557
V6 Mn1 V4 175.40(10) . 10_557
V7 Mn1 V4 95.11(8) . 10_557
V7 Mn1 V4 63.60(6) 10_557 10_557
V4 Mn1 V4 62.59(8) . 10_557
O20 V3 O20 106.5(6) . 10_557
O20 V3 O23 100.0(3) . .
O20 V3 O23 100.0(3) 10_557 .
O20 V3 O22 99.7(3) . .
O20 V3 O22 99.7(3) 10_557 .
O23 V3 O22 146.7(4) . .
O20 V3 O21 162.8(4) . 10_557
O20 V3 O21 90.7(3) 10_557 10_557
O23 V3 O21 76.9(3) . 10_557
O22 V3 O21 76.3(3) . 10_557
O20 V3 O21 90.7(3) . .
O20 V3 O21 162.8(4) 10_557 .
O23 V3 O21 76.9(3) . .
O22 V3 O21 76.3(3) . .
O21 V3 O21 72.2(4) 10_557 .
O20 V3 Mn1 126.8(3) . .
O20 V3 Mn1 126.8(3) 10_557 .
O23 V3 Mn1 73.6(3) . .
O22 V3 Mn1 73.1(3) . .
O21 V3 Mn1 36.08(18) 10_557 .
O21 V3 Mn1 36.08(18) . .
O20 V3 K1 53.8(3) . .
O20 V3 K1 53.8(3) 10_557 .
O23 V3 K1 97.2(4) . .
O22 V3 K1 116.1(4) . .
O21 V3 K1 142.95(19) 10_557 .
O21 V3 K1 142.95(19) . .
Mn1 V3 K1 170.8(2) . .
O20 V3 K1 71.5(3) . 3_565
O20 V3 K1 71.5(3) 10_557 3_565
O23 V3 K1 164.9(4) . 3_565
O22 V3 K1 48.4(3) . 3_565
O21 V3 K1 114.9(2) 10_557 3_565
O21 V3 K1 114.9(2) . 3_565
Mn1 V3 K1 121.5(2) . 3_565
K1 V3 K1 67.7(4) . 3_565
O15 V4 O19 106.3(4) . .
O15 V4 O18 101.8(4) . .
O19 V4 O18 96.6(4) . .
O15 V4 O22 99.1(4) . .
O19 V4 O22 95.9(4) . .
O18 V4 O22 151.5(4) . .
O15 V4 O21 95.6(3) . .
O19 V4 O21 157.9(3) . .
O18 V4 O21 81.6(3) . .
O22 V4 O21 77.3(3) . .
O15 V4 O16 169.2(4) . .
O19 V4 O16 84.2(4) . .
O18 V4 O16 79.2(3) . .
O22 V4 O16 76.8(3) . .
O21 V4 O16 73.8(3) . .
O15 V4 Mn1 133.0(3) . .
O19 V4 Mn1 120.7(3) . .
O18 V4 Mn1 76.7(2) . .
O22 V4 Mn1 74.9(3) . .
O21 V4 Mn1 37.37(19) . .
O16 V4 Mn1 36.5(3) . .
O15 V4 K1 69.3(3) . 3_565
O19 V4 K1 80.6(3) . 3_565
O18 V4 K1 169.2(3) . 3_565
O22 V4 K1 39.2(3) . 3_565
O21 V4 K1 105.0(3) . 3_565
O16 V4 K1 110.8(2) . 3_565
Mn1 V4 K1 113.74(13) . 3_565
O17 V5 O14 106.8(4) . .
O17 V5 O12 101.8(4) . .
O14 V5 O12 96.8(4) . .
O17 V5 O23 99.3(4) . .
O14 V5 O23 95.5(4) . .
O12 V5 O23 151.3(4) . .
O17 V5 O21 95.2(3) . .
O14 V5 O21 157.8(3) . .
O12 V5 O21 81.1(3) . .
O23 V5 O21 77.8(3) . .
O17 V5 O13 168.9(4) . .
O14 V5 O13 84.2(4) . .
O12 V5 O13 78.3(3) . .
O23 V5 O13 77.2(3) . .
O21 V5 O13 73.8(3) . .
O17 V5 Mn1 132.5(3) . .
O14 V5 Mn1 120.7(3) . .
O12 V5 Mn1 76.1(2) . .
O23 V5 Mn1 75.3(3) . .
O21 V5 Mn1 37.31(19) . .
O13 V5 Mn1 36.5(3) . .
O17 V5 V10 141.9(3) . .
O14 V5 V10 35.2(3) . .
O12 V5 V10 86.0(2) . .
O23 V5 V10 89.2(3) . .
O21 V5 V10 122.9(2) . .
O13 V5 V10 49.1(3) . .
Mn1 V5 V10 85.60(8) . .
O7 V6 O10 103.9(4) . .
O7 V6 O5 104.1(4) . .
O10 V6 O5 94.0(5) . .
O7 V6 O12 101.6(4) . .
O10 V6 O12 89.4(3) . .
O5 V6 O12 152.4(4) . .
O7 V6 O9 100.8(4) . .
O10 V6 O9 154.1(3) . .
O5 V6 O9 87.2(4) . .
O12 V6 O9 78.1(3) . .
O7 V6 O13 175.0(4) . .
O10 V6 O13 80.3(4) . .
O5 V6 O13 78.2(3) . .
O12 V6 O13 75.5(3) . .
O9 V6 O13 74.7(3) . .
O7 V6 V11 89.2(4) . .
O10 V6 V11 132.6(4) . .
O5 V6 V11 38.7(4) . .
O12 V6 V11 132.8(4) . .
O9 V6 V11 54.7(4) . .
O13 V6 V11 89.9(3) . .
O7 V6 Mn1 138.6(4) . .
O10 V6 Mn1 117.3(3) . .
O5 V6 Mn1 78.1(3) . .
O12 V6 Mn1 76.0(2) . .
O9 V6 Mn1 37.8(2) . .
O13 V6 Mn1 37.1(3) . .
V11 V6 Mn1 66.5(3) . .
O7 V6 V8 89.0(3) . .
O10 V6 V8 126.4(3) . .
O5 V6 V8 133.3(4) . .
O12 V6 V8 37.1(2) . .
O9 V6 V8 46.1(2) . .
O13 V6 V8 86.2(2) . .
V11 V6 V8 98.6(3) . .
Mn1 V6 V8 63.95(6) . .
O7 V6 V10 135.3(4) . .
O10 V6 V10 31.5(3) . .
O5 V6 V10 83.5(4) . .
O12 V6 V10 85.4(2) . .
O9 V6 V10 123.7(2) . .
O13 V6 V10 49.0(3) . .
V11 V6 V10 118.13(19) . .
Mn1 V6 V10 86.05(8) . .
V8 V6 V10 117.85(9) . .
O6 V7 O8 103.9(4) . .
O6 V7 O3 103.4(4) . .
O8 V7 O3 93.3(4) . .
O6 V7 O18 102.2(4) . .
O8 V7 O18 89.7(3) . .
O3 V7 O18 152.7(4) . .
O6 V7 O9 100.8(4) . .
O8 V7 O9 154.4(3) . .
O3 V7 O9 87.5(4) . .
O18 V7 O9 78.5(3) . .
O6 V7 O16 175.1(4) . .
O8 V7 O16 80.4(4) . .
O3 V7 O16 78.5(3) . .
O18 V7 O16 75.3(3) . .
O9 V7 O16 74.6(3) . .
O6 V7 V11 88.9(4) . .
O8 V7 V11 132.1(4) . .
O3 V7 V11 39.0(4) . .
O18 V7 V11 133.0(4) . .
O9 V7 V11 54.5(4) . .
O16 V7 V11 89.9(3) . .
O6 V7 Mn1 138.5(4) . .
O8 V7 Mn1 117.4(3) . .
O3 V7 Mn1 78.4(3) . .
O18 V7 Mn1 76.2(2) . .
O9 V7 Mn1 37.8(2) . .
O16 V7 Mn1 37.0(3) . .
V11 V7 Mn1 66.4(3) . .
O6 V7 V8 89.4(3) . .
O8 V7 V8 127.0(3) . .
O3 V7 V8 133.7(4) . .
O18 V7 V8 37.4(2) . .
O9 V7 V8 46.2(2) . .
O16 V7 V8 86.1(2) . .
V11 V7 V8 98.5(3) . .
Mn1 V7 V8 63.95(6) . .
O6 V7 V9 135.4(4) . .
O8 V7 V9 31.6(3) . .
O3 V7 V9 83.2(3) . .
O18 V7 V9 85.3(2) . .
O9 V7 V9 123.7(2) . .
O16 V7 V9 49.1(3) . .
V11 V7 V9 117.98(19) . .
Mn1 V7 V9 86.06(8) . .
V8 V7 V9 117.99(9) . .
O2 V8 O11 105.9(5) . .
O2 V8 O12 101.6(4) . .
O11 V8 O12 100.9(4) . .
O2 V8 O18 101.9(4) . .
O11 V8 O18 100.1(4) . .
O12 V8 O18 142.7(3) . .
O2 V8 O9 96.9(4) . .
O11 V8 O9 157.2(4) . .
O12 V8 O9 74.0(3) . .
O18 V8 O9 74.7(3) . .
O2 V8 O21 166.5(4) . .
O11 V8 O21 87.6(4) . .
O12 V8 O21 75.2(3) . .
O18 V8 O21 75.2(3) . .
O9 V8 O21 69.6(2) . .
O2 V8 V7 87.3(4) . .
O11 V8 V7 138.4(3) . .
O12 V8 V7 115.2(2) . .
O18 V8 V7 38.3(2) . .
O9 V8 V7 41.2(2) . .
O21 V8 V7 82.50(18) . .
O2 V8 V6 87.2(4) . .
O11 V8 V6 138.7(3) . .
O12 V8 V6 37.9(2) . .
O18 V8 V6 115.6(2) . .
O9 V8 V6 40.9(2) . .
O21 V8 V6 82.42(18) . .
V7 V8 V6 79.81(7) . .
O4 V9 O8 104.0(4) . 10_557
O4 V9 O8 104.0(4) . .
O8 V9 O8 92.5(5) 10_557 .
O4 V9 O19 101.5(4) . .
O8 V9 O19 153.8(4) 10_557 .
O8 V9 O19 86.9(3) . .
O4 V9 O19 101.5(4) . 10_557
O8 V9 O19 86.9(3) 10_557 10_557
O8 V9 O19 153.8(4) . 10_557
O19 V9 O19 82.4(5) . 10_557
O4 V9 O16 175.3(6) . .
O8 V9 O16 79.1(3) 10_557 .
O8 V9 O16 79.1(3) . .
O19 V9 O16 75.1(3) . .
O19 V9 O16 75.1(3) 10_557 .
O4 V9 V7 135.5(4) . 10_557
O8 V9 V7 31.5(2) 10_557 10_557
O8 V9 V7 83.0(3) . 10_557
O19 V9 V7 122.9(2) . 10_557
O19 V9 V7 83.0(2) 10_557 10_557
O16 V9 V7 47.84(18) . 10_557
O4 V9 V7 135.5(4) . .
O8 V9 V7 83.0(3) 10_557 .
O8 V9 V7 31.5(2) . .
O19 V9 V7 83.0(2) . .
O19 V9 V7 122.9(2) 10_557 .
O16 V9 V7 47.84(18) . .
V7 V9 V7 60.70(10) 10_557 .
O1 V10 O10 104.0(4) . 10_557
O1 V10 O10 104.0(4) . .
O10 V10 O10 92.7(5) 10_557 .
O1 V10 O14 101.9(5) . .
O10 V10 O14 153.4(4) 10_557 .
O10 V10 O14 86.8(3) . .
O1 V10 O14 101.9(5) . 10_557
O10 V10 O14 86.8(3) 10_557 10_557
O10 V10 O14 153.4(4) . 10_557
O14 V10 O14 82.1(5) . 10_557
O1 V10 O13 176.2(6) . .
O10 V10 O13 78.5(3) 10_557 .
O10 V10 O13 78.5(3) . .
O14 V10 O13 75.3(3) . .
O14 V10 O13 75.3(3) 10_557 .
O1 V10 V6 135.1(4) . 10_557
O10 V10 V6 31.2(2) 10_557 10_557
O10 V10 V6 82.7(3) . 10_557
O14 V10 V6 122.9(2) . 10_557
O14 V10 V6 83.2(2) 10_557 10_557
O13 V10 V6 47.63(19) . 10_557
O1 V10 V6 135.1(4) . .
O10 V10 V6 82.7(3) 10_557 .
O10 V10 V6 31.2(2) . .
O14 V10 V6 83.2(2) . .
O14 V10 V6 122.9(2) 10_557 .
O13 V10 V6 47.63(19) . .
V6 V10 V6 60.46(10) 10_557 .
O1 V10 V5 131.7(4) . .
O10 V10 V5 124.1(3) 10_557 .
O10 V10 V5 79.7(2) . .
O14 V10 V5 29.8(2) . .
O14 V10 V5 78.7(2) 10_557 .
O13 V10 V5 45.60(18) . .
V6 V10 V5 93.19(9) 10_557 .
V6 V10 V5 62.67(7) . .
O1 V10 V5 131.7(4) . 10_557
O10 V10 V5 79.7(2) 10_557 10_557
O10 V10 V5 124.1(3) . 10_557
O14 V10 V5 78.7(2) . 10_557
O14 V10 V5 29.8(2) 10_557 10_557
O13 V10 V5 45.60(18) . 10_557
V6 V10 V5 62.67(7) 10_557 10_557
V6 V10 V5 93.19(9) . 10_557
V5 V10 V5 61.49(9) . 10_557
V3 O23 V5 107.6(3) . 10_557
V3 O23 V5 107.6(3) . .
V5 O23 V5 109.7(5) 10_557 .
V3 O22 V4 108.1(3) . 10_557
V3 O22 V4 108.1(3) . .
V4 O22 V4 109.8(5) 10_557 .
V3 O22 K1 100.7(5) . 3_565
V4 O22 K1 114.7(3) 10_557 3_565
V4 O22 K1 114.7(3) . 3_565
Mn1 O21 V5 98.5(3) . .
Mn1 O21 V4 98.4(3) . .
V5 O21 V4 162.5(4) . .
Mn1 O21 V3 99.8(3) . .
V5 O21 V3 90.5(3) . .
V4 O21 V3 91.0(3) . .
Mn1 O21 V8 98.7(3) . .
V5 O21 V8 86.6(3) . .
V4 O21 V8 86.4(3) . .
V3 O21 V8 161.6(3) . .
V3 O20 Ce1 135.8(4) . .
V3 O20 K1 99.1(4) . .
Ce1 O20 K1 124.0(3) . .
V4 O19 V9 115.0(4) . .
V4 O18 V8 108.7(3) . .
V4 O18 V7 112.2(4) . .
V8 O18 V7 104.3(3) . .
V5 O17 Ce1 131.5(4) . .
Mn1 O16 V4 97.6(3) . .
Mn1 O16 V4 97.6(3) . 10_557
V4 O16 V4 91.6(4) . 10_557
Mn1 O16 V7 93.7(3) . 10_557
V4 O16 V7 168.1(5) . 10_557
V4 O16 V7 90.47(9) 10_557 10_557
Mn1 O16 V7 93.7(3) . .
V4 O16 V7 90.47(9) . .
V4 O16 V7 168.1(5) 10_557 .
V7 O16 V7 85.1(3) 10_557 .
Mn1 O16 V9 175.6(5) . .
V4 O16 V9 85.4(3) . .
V4 O16 V9 85.4(3) 10_557 .
V7 O16 V9 83.0(3) 10_557 .
V7 O16 V9 83.0(3) . .
V4 O15 Ce1 131.0(4) . .
V5 O14 V10 115.0(4) . .
Mn1 O13 V5 97.4(3) . 10_557
Mn1 O13 V5 97.4(3) . .
V5 O13 V5 91.0(4) 10_557 .
Mn1 O13 V6 93.9(4) . 10_557
V5 O13 V6 90.79(9) 10_557 10_557
V5 O13 V6 168.3(5) . 10_557
Mn1 O13 V6 93.9(4) . .
V5 O13 V6 168.3(5) 10_557 .
V5 O13 V6 90.79(9) . .
V6 O13 V6 85.2(3) 10_557 .
Mn1 O13 V10 176.2(6) . .
V5 O13 V10 85.3(3) 10_557 .
V5 O13 V10 85.3(3) . .
V6 O13 V10 83.3(3) 10_557 .
V6 O13 V10 83.3(3) . .
V5 O12 V8 108.5(3) . .
V5 O12 V6 112.5(4) . .
V8 O12 V6 105.0(4) . .
V8 O11 Ce1 140.4(5) . .
V6 O10 V10 117.3(4) . .
Mn1 O9 V6 101.4(3) . .
Mn1 O9 V7 101.2(3) . .
V6 O9 V7 154.7(4) . .
Mn1 O9 V8 103.3(3) . .
V6 O9 V8 93.0(3) . .
V7 O9 V8 92.6(3) . .
Mn1 O9 V11 97.8(4) . .
V6 O9 V11 83.0(5) . .
V7 O9 V11 83.0(5) . .
V8 O9 V11 158.9(4) . .
V7 O8 V9 116.9(4) . .
V6 O5 V6 117.0(6) . 10_557
V6 O5 V11 105.0(5) . .
V6 O5 V11 105.0(5) 10_557 .
V7 O3 V7 116.6(6) . 10_557
V7 O3 V11 104.5(5) . .
V7 O3 V11 104.5(5) 10_557 .
S1 O5W Ce1 140.2(5) . .
O25 S1 O5W 109.7(5) . 2_665
O25 S1 O5W 109.7(5) . 3_565
O5W S1 O5W 109.2(5) 2_665 3_565
O25 S1 O5W 109.7(5) . .
O5W S1 O5W 109.2(5) 2_665 .
O5W S1 O5W 109.2(5) 3_565 .
O25 S1 K1 38.46(15) . .
O5W S1 K1 79.2(5) 2_665 .
O5W S1 K1 144.4(5) 3_565 .
O5W S1 K1 99.6(5) . .
O25 S1 K1 38.46(16) . 2_665
O5W S1 K1 99.6(5) 2_665 2_665
O5W S1 K1 79.2(5) 3_565 2_665
O5W S1 K1 144.4(5) . 2_665
K1 S1 K1 65.2(2) . 2_665
O25 S1 K1 38.46(15) . 3_565
O5W S1 K1 144.4(5) 2_665 3_565
O5W S1 K1 99.6(5) 3_565 3_565
O5W S1 K1 79.2(5) . 3_565
K1 S1 K1 65.2(2) . 3_565
K1 S1 K1 65.2(2) 2_665 3_565
S1 O25 K1 122.7(4) . .
S1 O25 K1 122.7(4) . 2_665
K1 O25 K1 93.6(5) . 2_665
S1 O25 K1 122.7(4) . 3_565
K1 O25 K1 93.6(5) . 3_565
K1 O25 K1 93.6(5) 2_665 3_565
O51 C1 O51 121(2) 10_556 .
O51 C1 C2 119.5(11) 10_556 .
O51 C1 C2 119.5(11) . .
C3 C2 C3 120.9(13) . 10_556
C3 C2 C1 119.5(6) . .
C3 C2 C1 119.5(6) 10_556 .
C3 C4 C5 120.7(11) . .
C4 C3 C2 119.2(12) . .
N1 C5 C4 0(3) 10_556 10_556
N1 C5 C4 119.3(11) 10_556 .
C4 C5 C4 119.3(11) 10_556 .
O53 V11 O53 69(3) 10_557 .
O53 V11 O5 106.5(17) 10_557 .
O53 V11 O5 106.5(17) . .
O53 V11 O3 105.9(17) 10_557 .
O53 V11 O3 105.9(17) . .
O5 V11 O3 140.5(10) . .
O53 V11 O9 179.5(16) 10_557 .
O53 V11 O9 111.0(15) . .
O5 V11 O9 73.6(6) . .
O3 V11 O9 74.2(6) . .
O53 V11 O9 111.0(15) 10_557 10_557
O53 V11 O9 179.5(16) . 10_557
O5 V11 O9 73.6(6) . 10_557
O3 V11 O9 74.2(6) . 10_557
O9 V11 O9 69.6(6) . 10_557
O53 V11 V6 137.6(17) 10_557 .
O53 V11 V6 98.6(15) . .
O5 V11 V6 36.3(3) . .
O3 V11 V6 116.5(6) . .
O9 V11 V6 42.3(3) . .
O9 V11 V6 81.8(5) 10_557 .
O53 V11 V6 98.6(15) 10_557 10_557
O53 V11 V6 137.6(17) . 10_557
O5 V11 V6 36.3(3) . 10_557
O3 V11 V6 116.5(6) . 10_557
O9 V11 V6 81.8(5) . 10_557
O9 V11 V6 42.3(3) 10_557 10_557
V6 V11 V6 63.0(3) . 10_557
O53 V11 V7 137.4(17) 10_557 .
O53 V11 V7 98.5(16) . .
O5 V11 V7 116.1(7) . .
O3 V11 V7 36.5(3) . .
O9 V11 V7 42.5(3) . .
O9 V11 V7 81.9(5) 10_557 .
V6 V11 V7 83.0(3) . .
V6 V11 V7 115.1(5) 10_557 .
O53 V11 V7 98.5(16) 10_557 10_557
O53 V11 V7 137.4(17) . 10_557
O5 V11 V7 116.1(7) . 10_557
O3 V11 V7 36.5(3) . 10_557
O9 V11 V7 81.9(5) . 10_557
O9 V11 V7 42.5(3) 10_557 10_557
V6 V11 V7 115.1(5) . 10_557
V6 V11 V7 83.0(3) 10_557 10_557
V7 V11 V7 63.0(4) . 10_557
O25 K1 O25 65.3(8) . 10_557
O25 K1 O22 111.6(4) . 2_665
O25 K1 O22 111.6(4) 10_557 2_665
O25 K1 O20 99.2(4) . 10_557
O25 K1 O20 70.9(3) 10_557 10_557
O22 K1 O20 147.2(3) 2_665 10_557
O25 K1 O20 70.9(3) . .
O25 K1 O20 99.2(4) 10_557 .
O22 K1 O20 147.2(3) 2_665 .
O20 K1 O20 53.7(4) 10_557 .
O25 K1 V3 87.7(3) . .
O25 K1 V3 87.7(3) 10_557 .
O22 K1 V3 156.8(5) 2_665 .
O20 K1 V3 27.07(19) 10_557 .
O20 K1 V3 27.07(19) . .
O25 K1 V3 85.8(3) . 2_665
O25 K1 V3 85.8(3) 10_557 2_665
O22 K1 V3 30.9(2) 2_665 2_665
O20 K1 V3 151.0(2) 10_557 2_665
O20 K1 V3 151.0(2) . 2_665
V3 K1 V3 172.3(4) . 2_665
O25 K1 S1 18.9(4) . .
O25 K1 S1 84.2(5) 10_557 .
O22 K1 S1 105.8(3) 2_665 .
O20 K1 S1 107.0(3) 10_557 .
O20 K1 S1 65.5(2) . .
V3 K1 S1 88.3(2) . .
V3 K1 S1 86.9(2) 2_665 .
O25 K1 S1 84.2(5) . 10_557
O25 K1 S1 18.9(4) 10_557 10_557
O22 K1 S1 105.8(3) 2_665 10_557
O20 K1 S1 65.5(2) 10_557 10_557
O20 K1 S1 107.0(3) . 10_557
V3 K1 S1 88.3(2) . 10_557
V3 K1 S1 86.9(2) 2_665 10_557
S1 K1 S1 103.1(3) . 10_557
O25 K1 V4 105.2(3) . 2_665
O25 K1 V4 133.5(4) 10_557 2_665
O22 K1 V4 26.08(12) 2_665 2_665
O20 K1 V4 151.3(4) 10_557 2_665
O20 K1 V4 121.3(2) . 2_665
V3 K1 V4 138.6(3) . 2_665
V3 K1 V4 47.71(14) 2_665 2_665
S1 K1 V4 92.35(15) . 2_665
S1 K1 V4 131.4(3) 10_557 2_665
O25 K1 V4 133.5(4) . 11_667
O25 K1 V4 105.2(3) 10_557 11_667
O22 K1 V4 26.08(12) 2_665 11_667
O20 K1 V4 121.3(2) 10_557 11_667
O20 K1 V4 151.3(4) . 11_667
V3 K1 V4 138.6(3) . 11_667
V3 K1 V4 47.71(14) 2_665 11_667
S1 K1 V4 131.4(3) . 11_667
S1 K1 V4 92.35(15) 10_557 11_667
V4 K1 V4 46.64(14) 2_665 11_667
O25 K1 K1 43.2(3) . 2_665
O25 K1 K1 43.2(3) 10_557 2_665
O22 K1 K1 85.9(5) 2_665 2_665
O20 K1 K1 111.0(3) 10_557 2_665
O20 K1 K1 111.0(3) . 2_665
V3 K1 K1 117.3(3) . 2_665
V3 K1 K1 55.0(3) 2_665 2_665
S1 K1 K1 57.41(12) . 2_665
S1 K1 K1 57.41(12) 10_557 2_665
V4 K1 K1 97.3(4) 2_665 2_665
V4 K1 K1 97.3(4) 11_667 2_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 O11 2.474(9) .
Ce1 O5W 2.481(9) .
Ce1 O4W 2.507(12) .
Ce1 O2W 2.518(11) .
Ce1 O1W 2.526(13) .
Ce1 O3W 2.532(11) .
Ce1 O20 2.582(9) .
Ce1 O17 2.608(8) .
Ce1 O15 2.630(8) .
Mn1 O16 1.845(10) .
Mn1 O13 1.846(10) .
Mn1 O21 1.886(7) .
Mn1 O21 1.886(7) 10_557
Mn1 O9 1.913(7) 10_557
Mn1 O9 1.913(7) .
Mn1 V6 3.057(3) 10_557
Mn1 V6 3.057(3) .
Mn1 V7 3.060(3) .
Mn1 V7 3.060(3) 10_557
Mn1 V4 3.074(3) .
Mn1 V4 3.074(3) 10_557
V3 O20 1.655(8) .
V3 O20 1.655(8) 10_557
V3 O23 1.921(10) .
V3 O22 1.925(10) .
V3 O21 2.231(7) 10_557
V3 O21 2.231(7) .
V3 K1 3.590(12) .
V3 K1 3.687(12) 3_565
V4 O15 1.617(8) .
V4 O19 1.714(8) .
V4 O18 1.908(7) .
V4 O22 1.952(6) .
V4 O21 2.169(7) .
V4 O16 2.227(7) .
V4 K1 4.034(11) 3_565
V5 O17 1.628(8) .
V5 O14 1.711(8) .
V5 O12 1.924(8) .
V5 O23 1.950(6) .
V5 O21 2.169(7) .
V5 O13 2.236(7) .
V5 V10 3.119(3) .
V6 O7 1.580(8) .
V6 O10 1.814(8) .
V6 O5 1.839(6) .
V6 O12 1.975(8) .
V6 O9 2.035(8) .
V6 O13 2.316(7) .
V6 V11 3.001(15) .
V6 V8 3.105(3) .
V6 V10 3.113(3) .
V7 O6 1.586(9) .
V7 O8 1.823(8) .
V7 O3 1.849(6) .
V7 O18 1.986(8) .
V7 O9 2.046(8) .
V7 O16 2.324(7) .
V7 V11 3.008(15) .
V7 V8 3.102(3) .
V7 V9 3.112(3) .
V8 O2 1.607(9) .
V8 O11 1.663(9) .
V8 O12 1.938(8) .
V8 O18 1.943(8) .
V8 O9 2.241(8) .
V8 O21 2.394(7) .
V9 O4 1.584(12) .
V9 O8 1.827(9) 10_557
V9 O8 1.827(9) .
V9 O19 1.981(8) .
V9 O19 1.981(8) 10_557
V9 O16 2.370(10) .
V9 V7 3.112(3) 10_557
V10 O1 1.591(12) .
V10 O10 1.831(9) 10_557
V10 O10 1.831(9) .
V10 O14 1.983(9) .
V10 O14 1.983(9) 10_557
V10 O13 2.367(10) .
V10 V6 3.113(3) 10_557
V10 V5 3.119(3) 10_557
O23 V5 1.950(6) 10_557
O22 V4 1.952(6) 10_557
O22 K1 2.807(15) 3_565
O20 K1 2.935(13) .
O16 V4 2.227(7) 10_557
O16 V7 2.324(7) 10_557
O13 V5 2.236(7) 10_557
O13 V6 2.316(7) 10_557
O9 V11 2.468(16) .
O5 V6 1.839(6) 10_557
O5 V11 1.94(2) .
O3 V7 1.849(6) 10_557
O3 V11 1.95(2) .
O5W S1 1.459(9) .
S1 O25 1.45(2) .
S1 O5W 1.459(9) 2_665
S1 O5W 1.459(9) 3_565
S1 K1 3.761(9) .
S1 K1 3.761(9) 2_665
S1 K1 3.761(9) 3_565
O25 K1 2.779(15) .
O25 K1 2.779(15) 2_665
O25 K1 2.779(15) 3_565
O51 C1 1.300(9) .
C1 O51 1.300(9) 10_556
C1 C2 1.459(10) .
C2 C3 1.403(10) .
C2 C3 1.403(10) 10_556
C4 C3 1.393(10) .
C4 C5 1.404(10) .
C5 N1 1.404(10) 10_556
C5 C4 1.404(10) 10_556
V11 O53 1.65(4) 10_557
V11 O53 1.65(4) .
V11 O9 2.468(16) 10_557
V11 V6 3.001(15) 10_557
V11 V7 3.008(15) 10_557
K1 O25 2.779(15) 10_557
K1 O22 2.807(15) 2_665
K1 O20 2.935(13) 10_557
K1 V3 3.687(12) 2_665
K1 S1 3.761(9) 10_557
K1 V4 4.034(11) 2_665
K1 V4 4.034(11) 11_667
K1 K1 4.05(2) 2_665
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 0.000 0.500 -0.002 1539.7 108.3
